- Nano Express
- Open Access
Attachment of Li[Ni0.2Li0.2Mn0.6]O2 Nanoparticles to the Graphene Surface Using Electrostatic Interaction Without Deterioration of Phase Integrity
Nanoscale Research Lettersvolume 11, Article number: 272 (2016)
In this article, we report a facile approach to enhance the electrochemical performance of Li-rich oxides with vulnerable phase stability. The Li-rich oxide nanoparticles were attached to the surface of graphene; the graphene surface acted as a matrix with high electronic conductivity that compensated for the low conductivity and enhanced the rate capability of the oxides. Our novel approach constitutes a direct assembly of two materials via electrostatic interaction, without a high-temperature heat treatment. The inevitable deterioration in phase integrity of previous composites between carbon and Li-rich oxides resulted from the reaction of oxygen in the structure with carbon during the heat-treatment process. However, our new method successfully attached Li-rich nanoparticles to the surface of graphene, without a phase change of the oxides. The resulting graphene/Li-rich oxide composites exhibited superior capacity and rate capability compared to their pristine Li-rich counterparts.
Recently, Li-ion batteries have been used as the main energy storage system for electrical devices and electrical vehicles [1–5]. However, the energy densities of commercial Li-ion batteries using LiCoO2 as a cathode cannot satisfy the demand of many of these applications [6–10]; new high-capacity cathode materials are therefore required. The layered Li-rich materials in the Li-Mn-Ni oxide system, which have higher energy densities (~250 mAh g−1) than other cathode materials such as LiCoO2 [11–18], have attracted significant attention as promising new cathode materials. However, major drawbacks such as poor rate capability owing to insufficient electronic and ionic conductivities [19–21] have prevented their use in commercial applications. Many attempts have been made to enhance the rate capability of the cathode-like Li-rich layered oxide. For example, compositing the oxide with carbon-based materials that have high electronic conductivity has been used as a means of compensating for the low conductivity of the cathode materials [22–25]. In fact, graphene comprising two-dimensional carbon sheets has been used as a novel matrix in cathode/carbon composites that have high rate capability and stable cyclic performance; the use of graphene stems from its excellent electronic conductivity and mechanical flexibility as well as high specific surface area [26–29]. However, compositing with carbon materials (such as graphene) requires high-temperature (greater than ~400 °C) heat-treatment processes that produce strong bonds between the cathode and carbon. Unfortunately, Li-rich layered oxides are susceptible to phase changes and deterioration of the structural integrity during processing; this deterioration results from the reaction of carbon with oxygen (at over 400 °C) and the consequent loss of oxygen from the structure of the oxides [28, 29]. Since most of the cathode materials, such as LiCoO2, LiFePO4, and LiMn2O4, are relatively stable during the heating process [22–27], this susceptibility to deterioration is attributed to the structural instability of the oxides.
To overcome this drawback, we propose a new method for the heat-treatment-free fabrication of composites between graphene and unstable Li-rich layered oxides. Our novel strategy for the composition relies on the electrostatic interaction of the two species. As illustrated in Fig. 1, the graphene particles and Li-rich layered oxides can be negatively and positively charged, respectively, by controlling the pH of the solution. These inversely charged particles induce a self-assembly between the graphene and the oxides via electrostatic interactions. This method is especially attractive because the graphene/cathode composite can be prepared through a simple drying process, without a high-temperature heat treatment. As such, the loss of oxygen is prevented and the phase and structural integrity of the vulnerable Li-rich layered oxides are maintained. In this work, Li[Ni0.2Li0.2Mn0.6]O2 nanoparticles (a typical Li-rich layered oxide) attached to the graphene surface were prepared via electrostatic interaction and tested as a cathode material for enhanced Li batteries.
Li[Ni0.2Li0.2Mn0.6]O2 nanoparticles were prepared via the general combustion method using a dispersing agent to control the particle size of the cathode powder . The prepared Li[Ni0.2Li0.2Mn0.6]O2 nanoparticles were composited with graphene via electrostatic interactions. The commercial graphene (AMG Graphite/Graphit Kropfmühl) was immersed into the 1-N acidic solution (nitric acid/sulfuric acid = 3:1) for 2 h for surface modification and washed several times using distilled water. Then the Li[Ni0.2Li0.2Mn0.6]O2 and graphene particles were dispersed in an ethanol-based solution by ultra-sonication; the weight % of the graphene to the Li[Ni0.2Li0.2Mn0.6]O2 was controlled to amounts of 0.5, 2.0, and 5.0. The pH of the solution was adjusted to 4 using buffer solution (pH 4) in order to control the surface potential of the graphene and the Li[Ni0.2Li0.2Mn0.6]O2 particles. After a 10-min stirring for homogeneous mixing, the solution was vacuum filtered and the resulting samples were dried at 200 °C for 2 h under an air atmosphere. X-ray diffraction (XRD) measurements were then performed on the samples with a Rigaku X-ray diffractometer using monochromatized Cu-Kα radiation (λ = 1.5406 Å). In addition, the surface of the Li[Ni0.2Li0.2Mn0.6]O2 nanoparticle/graphene composite was examined using a transmission electron microscope (TEM, JEOL-4010) and X-ray photoelectron spectroscopy (XPS, PHI 5000 VersaProbe, Ulvac-PHI). The C content of the composites was determined via thermogravimetric analysis (TGA, Q500 V20.13 Build 39) by heating from 200 to 750 °C under an air atmosphere.
For electrochemical testing, a cathode slurry was prepared by mixing Li[Ni0.2Li0.2Mn0.6]O2 nanoparticle/graphene composite (or pristine Li[Ni0.2Li0.2Mn0.6]O2 nanoparticles) and carbon black (Super P) with polyvinylidene fluoride (PVDF) in a weight ratio of 80 (cathode):10 (super P):10(PVDF). After 24 h of ball-mill processing, the viscous slurry was coated onto an Al foil using a doctor blade and subsequently dried at 90 °C in an oven. A coin-type cell (2032) consisting of a cathode, Li-metal anode, separator (25 μm, SK Innovation), and an electrolyte (1 M LiPF6 in EC/DMC (1:1 vol%)) was used. The cells were subjected to galvanostatic cycling in the voltage range of 4.8–2.0 V and at various charge-discharge rates, using a WonATech voltammetry system. In addition, impedance measurements were performed by applying an AC voltage at an amplitude of 5 mV and a frequency range of 0.1 Hz to 100 KHz, using an electrochemical workstation (AMETEK, VersaSTAT 3).
Results and Discussion
An appropriate pH value must be selected in order to directly assemble composites of graphene and Li[Ni0.2Li0.2Mn0.6]O2 nanoparticles via electrostatic interaction. Therefore, the appropriate pH value of the surface charges of graphene and the Li[Ni0.2Li0.2Mn0.6]O2 nanoparticles was determined via zeta potential measurements. As Fig. 2a shows, the surface of graphene was negatively charged at pH values of 3–6. In contrast, the surface charge of the Li[Ni0.2Li0.2Mn0.6]O2 nanoparticle switched from positive (over 20 mV) to negative (−20 mV) with increasing pH value. The graphene and Li[Ni0.2Li0.2Mn0.6]O2 nanoparticles should be oppositely charged in order to trigger the mutual assembly via electrostatic interaction, and hence the pH value should be lower than 4. Figure 2a shows that the electrostatic interaction between the particles increased with decreasing pH value. However, the low pH resulted in reduced integrity of the nanoparticles owing to the vulnerable surface of the Li-rich oxide in the acidic environment. As such, we determined that a pH value of 4 was appropriate, because this was the highest value that allowed the formation of composites between the oppositely charged graphene and Li[Ni0.2Li0.2Mn0.6]O2 nanoparticles.
To determine the actual graphene content, the results of the TGA of the pristine and composite samples were measured and compared as shown in Fig. 2b. If the composite sample is prepared through a high-temperature heat treatment, then some of the graphene will evaporate during the process. However, our composite samples were dried at 200 °C without heat treatment, and hence the original amount of graphene was maintained during the fabrication process. As Fig. 2b shows, composite 0.5, composite 2.0, and composite 5.0 exhibit weight loss of ~0.5, 2.0, and 5.0 wt.%, respectively, when the samples are heated to 750 °C. This weight loss stems from the evaporation of carbon and is therefore an indicator of the carbon content of the composites.
Figure 3 shows SEM and TEM images of the pristine Li[Ni0.2Li0.2Mn0.6]O2 nanoparticles and composites of the graphene and Li[Ni0.2Li0.2Mn0.6]O2 nanoparticles. Hereafter, we refer to the Li[Ni0.2Li0.2Mn0.6]O2 nanoparticles attached to 0.5 wt.% graphene, 2.0 wt.% graphene, and 5.0 wt.% graphene (wt.% means weight percent of the Li[Ni0.2Li0.2Mn0.6]O2 nanoparticles) as composite 0.5, composite 2.0, and composite 5.0, respectively. The Li[Ni0.2Li0.2Mn0.6]O2 powder consists of 200~500-nm-sized nanoparticles (Fig. 3a, e). Figure 3b, f shows that composite 0.5 consists of Li[Ni0.2Li0.2Mn0.6]O2 particles that are successfully composited with graphene; i.e., the particles cover most of the graphene surface. However, many of the particles were aggregated and did not have direct contact with graphene owing to its low (only 0.5 wt.%) surface area. In contrast, the graphene surface of composite 2.0 was appropriately covered with Li[Ni0.2Li0.2Mn0.6]O2 nanoparticles, as shown in Fig. 3c, g. The nanoparticles seemed to be strongly attached to graphene, which has a high electronic conductivity. Figure 3d, h shows the image of composite 5.0. As the figure shows, the Li[Ni0.2Li0.2Mn0.6]O2 nanoparticles are well-attached to, but only sparsely populate graphene; i.e., the surface area of the graphene far exceeded that of the nanoparticles
As mentioned previously, we expected the Li[Ni0.2Li0.2Mn0.6]O2 particles in our composites to retain their structural integrity and phase; this assumption was deemed reasonable since the composites were assembled via electrostatic interaction, without the use of a high-temperature heat-treatment process that leads to oxygen loss and phase changes. To determine the validity of this assumption, the pristine sample and composites were evaluated via XRD and XPS measurements. Figure 4a compares the XRD patterns of the samples. The patterns (Fig. 4a) from the pristine sample and the composites were very similar and corresponded closely to that of the hexagonal α-NaFeO2 structure (space group R-3m); the peaks occurring at angles of 20°–25° are associated with superlattice ordering in the transition metal layers. The pattern was examined in further detail by enlarging the peaks occurring at angles of 18°–20°, 20°–30°, and 40°–50°. These peaks are associated with the (003), superlattice ordering and graphene, and (104) and (105) reflections, which are shown in Fig. 4b–d, respectively. Previous studies [28, 29] have shown that the diffraction pattern of carbon/Li-rich oxide composites (prepared via a heat-treatment process) differed somewhat from that of the pristine sample. There, the (003) peaks were shifted and peaks associated with the spinel-like phase occurred, owing to the effect of oxygen loss. However, in our work, the peaks corresponding to the pristine and composite samples were almost identical, indicating that the method of electrostatic interaction prevented the phase change of the vulnerable Li-rich oxide (Li[Ni0.2Li0.2Mn0.6]O2). As shown in Fig. 4c, the peaks corresponding to graphene are clearly detected in the patterns of the composites.
Figure 5 shows the XPS spectra of the O 1s, Li 1s, Mn 2p, and Ni 2p orbitals of the pristine and composite samples. The curves were all calibrated based on the C 1s (C–C bond) peak (284.5 eV). The XPS spectrum of the composite prepared via a heat-treatment process differed significantly from that of the pristine sample . Specifically, the intensity of TM-O (TM = transition metal such as Ni, Mn, Co) bond (~529.5 eV) was increased, and the intensity of Li 1s peak (~54.2 eV) was decreased. This indicates that compared to the pristine sample, the composites have higher and lower content of transition metal and Li, respectively, on their surface. Furthermore, this result is attributed to the phase transformation of the surface layer to the spinel-like (−LiMn2O4) phase; this phase has a higher transition metal (Mn) content and lower amounts of Li than the pristine Li-rich oxide (typically, the Li:Mn ratio is approximately 1.2:0.8). However, this phase transition did not occur in the composites prepared by our method of electrostatic interaction. The peaks corresponding to the TM–O (TM=Mn and Ni) bond (~529.5 eV) of the samples (Fig. 5a) exhibited similar intensities, although those of the C–O and C=O bonds increased with increasing C content of the composites. The peaks corresponding to the Li 1s (~54.2 eV) also exhibited (Fig. 5b) similar intensities in both the pristine and the composite samples. This indicates that the spinel-like phase did not form during the fabrication of the composites. Moreover, the peak corresponding to the Mn 3p and Mn 2p occurred in similar positions in both the pristine and composite samples, as shown in Fig. 5b, c. This indicates that the composites have similar Mn oxidation states as their pristine counterpart. Previous studies [28, 29] showed the Mn oxidation state of composites prepared via a heat-treatment process differed significantly from that of the pristine sample. The peaks related to Mn shifted, and the intensity of those was also changed due to composite-process. Therefore, the similarities observed in Fig. 5 are indicative of the phase integrity of our composites that are prepared by electrostatic interaction.
The effect of graphene as a matrix material was determined by evaluating the electrochemical properties of the pristine samples and the composites. Figure 6a shows the discharge capacities of the samples measured at current densities of 44, 110, 220, 660, and 1320 mA g−1, in a voltage range of 4.8–2.0 V. As the figure shows, the discharge capacities of the composites are all somewhat higher than that of the pristine sample. Composites 2.0 and 5.0 have, in particular, a higher discharge capacity and superior rate capability compared with those of composite 0.5. Table 1 summarizes the discharge capacities and capacity retentions of the samples measured at various current densities (3rd, 6th, 11th, 21st, and 31st cycles of Fig. 6a). The capacity retention of the pristine sample at 1320 mA g−1 was only ~44 % of that measured at a current density of 44 mA g−1. In contrast, composites 2.0 and 5.0 exhibited superior capacity retention of ~53 %. These improved electrochemical properties stem from the effect of graphene acting as a matrix for the Li[Ni0.2Li0.2Mn0.6]O2 nanoparticles; i.e., the high electronic conductivity of the graphene matrix compensates for the low conductivity of the Li[Ni0.2Li0.2Mn0.6]O2 nanoparticles, thereby leading to the enhanced electrochemical performance of the composite.
Figure 6b shows the results of electrochemical impedance spectroscopy measurements performed prior to the electrochemical tests. The Nyquist plots composed of a broad semicircle, which may be overlapped two semicircles. Generally, a semicircle located in high-frequency range represents the impedance due to a solid electrolyte interface, and a semicircle in relatively low-frequency range represents the charge-transfer resistance at the electrode/electrolyte interface [9, 30]. The size of the semicircle is dependent upon the impedance value of the cell. As shown in Fig. 6b, the semicircles associated with the composites had smaller diameters than the semicircle corresponding to the pristine sample. This indicates that graphene-containing composites are effective in reducing the impedance value of the Li[Ni0.2Li0.2Mn0.6]O2 cathode. Furthermore, the enhanced rate capability (Fig. 6a) of the composites results from this reduced impedance. The impedance value of the composite 5.0 was somewhat higher than composite 2.0, which may due to large amount of graphene. Too much graphene can block Li+ transport between liquid electrolyte and cathode surface since Li+ cannot penetrate through the graphene layer.
Figure 6c shows the cyclic performance of the samples measured at a current density of 110 mA g−1 and a voltage range of 4.8–2.0 V. The discharge capacity of the composites was somewhat higher than that of the pristine sample. However, the cyclic performance of the samples differed only slightly. The corresponding discharge profiles after various cycles (left in Fig. 7) reveal that the discharge capacities of the samples decrease gradually during cycling. More importantly, a double-plateau region did not form during cycling. These plateaus are indicative of the phase transformation from a layered structure of Li-rich oxides to a spinel-like structure, during cycling of the carbon/Li-rich oxide composite fabricated via a heat-treatment process [28, 29]. This transformation is attributed to the deterioration of phase integrity and the oxygen loss stemming from the reaction with C (graphene) during the fabrication process. However, the absence of these plateaus indicates that our composite, prepared by electrostatic interaction, maintained a stable phase during cycling; i.e., the compositing process did not reduce the phase integrity of the Li-rich oxide. This can be also confirmed by the dQ/dV plots in Fig. 7 (right side). The peaks in the samples shifted to the low potential during cycling. However, the sharp peak below 3.0 V, indicating the phase transformation to spinel [28, 29], was not growing during cycling. Therefore, the novel fabrication method described in this work constitutes an effective approach for maintaining phase integrity and enhancing the electrochemical performance of Li-rich oxides that consist of a vulnerable phase.
Li[Ni0.2Li0.2Mn0.6]O2 nanoparticles were successfully composited on the surface of graphene using electrostatic interaction without a high-temperature heat-treatment process. Carbon/Li-rich oxide composites (prepared via a heat-treatment process) are, in general, susceptible to phase changes and deterioration of the phase integrity; this deterioration results from the reaction of carbon with oxygen and consequent loss of oxygen from the structure of the vulnerable Li-rich oxide phase. However, we successfully fabricated graphene/Li[Ni0.2Li0.2Mn0.6]O2 composites using electrostatic interaction without deterioration of the phase integrity of the oxides, as confirmed by XRD and XPS analysis. The optimized graphene/Li[Ni0.2Li0.2Mn0.6]O2 composites (composite 2.0) exhibited higher discharge capacity and improved rate capability compared with those of pristine Li[Ni0.2Li0.2Mn0.6]O2. This improvement is attributed to the high conductivity of graphene, which compensates for the low conductivity of the pristine Li[Ni0.2Li0.2Mn0.6]O2.
Jin G, Qiao H, Xie H, Wang H, He K, Liu P, Chen J, Tang Y, Liu S, Huang C, Synthesis of single-crystalline octahedral LiMn2O4 as high performance cathode for Li-ion battery, (2014) Electrochim Acta 150:1
Najak PK, Grinblat J, Levi M, Aubach D, Electrochemical and structural characterization of carbon coated Li1.2Mn0.56Ni0.16Co0.08O2 and Li1.2Mn0.6Ni0.2O2 as cathode materials for Li-ion batteries, (2014) Electrochim Acta 137:556
Hutzenlaub T, Thiele S, Paust N, Spotnitz R, Zengerle R, Walchshofer C, Three-dimensional electrochemical Li-ion battery modelling featuring a focused ion-beam/scanning electron microscopy based three-phase reconstruction of a LiCoO2 cathode, (2014) Electrochim Acta 115:139
Lee HJ, Park KS, Park YJ,Surface modification of Li[Ni0.3Co0.4Mn0.3]O2 cathode by Li–La–Ti–O coating, (2010) J Power Sources 195:6122
Philippe B, Mahmoud A, Ledeuil JB, Sougrati MT, Edström K, Dedryvère R, Gonbeau D, Lippens P-E, MnSn2 electrodes for Li-ion batteries: Mechanisms at the nano scale and electrode/electrolyte interface, (2014) Electrochim Acta 123:72
Rad MS, Danilov DL, Baghalha M, Kazemeini M, Notten PHL, Adaptive thermal modeling of Li-ion batteries, (2013) Electrochim Acta 102:183
Song HG, Kim JY, Kim KT, Park YJ, Enhanced electrochemical properties of Li(Ni0.4Co0.3Mn0.3)O2 cathode by surface modification using Li3PO4-based materials, (2011) J Power Sources 196:6847
Dimov N, Nishimura A, Chihara K, Kitajou A, Gocheva ID, Okada S, Transition metal NaMF3 compounds as model systems for studying the feasibility of ternary Li-M-F and Na-M-F single phases as cathodes for lithium–ion and sodium–ion batteries, (2013) Electrochim Acta 110:214
Song HG, Kim JY, Park YJ, Enhanced electrochemical and storage properties of La2/3-x Li 3XTiO3-coated Li[Ni-coatedLi[Ni 0.4Co0.3Mn0.3]O2, (2011) Electrochim Acta 56:6896
Lu Z, Dahn JR, Understanding the Anomalous Capacity of Li / Li [ NixLi(1 / 3 − 2x / 3) Mn(2 / 3 − x / 3)] O2 Cells Using In Situ X-Ray Diffraction and Electrochemical Studies, (2002) J Electrochem Soc 149:A815
Arunkumar TA, Alvarez E, Manthiram A, Chemical and structural instability of the chemically delithiated (1 – z) Li[Li1/3Mn2/3]O2·(z) Li[Co1–yNiy]O2 (0 ≤ y ≤ 1 and 0 ≤ z ≤ 1) solid solution cathodes, (2008) J Mater Chem 18:190
Li J, Klöpsch R, Stan MC, Nowak S, Kunze M, Winter M, Passerini S, Synthesis and electrochemical performance of the high voltage cathode material Li[Li0.2Mn0.56Ni0.16Co0.08]O2 with improved rate capability, (2011) J Power Sources 196:4821
Hong YS, Park YJ, Ryu KS, Chang SH, Kim MG, Synthesis and electrochemical properties of nanocrystalline Li[NixLi(1−2x)/3Mn(2−x)/3]O2 prepared by a simple combustion method, J. Mater. Chem., (2004) J Mater Chem 14:1424
Ates MN, Jia Q, Shah A, Busnaina A, Mukerjee S, Abraham KM, Mitigation of layered to spinel conversion of a Li-rich layered metal oxide cathode material for Li-ion batteries, (2014) J Electrochem Soc 161:A290
Lee HJ, Park Y, Surface modification of Li[Li0.2Ni0.2Mn0.6]O2 nanoparticles with polydopamine-assisted MgF2 coating,J (2014) Mater Res Bull 58:169
Ates MN, Mukerjee S, Abraham KM, A Li-Rich Layered Cathode Material with Enhanced Structural Stability and Rate Capability for Li-on Batteries, (2014) J Electrochem Soc 161:A335
Tran HY, Taubert C, Fleischhammer M, Axmann P, Kuppers L, Wohlfahrt-Mehrens M, Chemical Lithiation Studies on Combustion Synthesized V2O5 Cathodes with Full Cell Application for Lithium Ion Batteries, (2013) J Electrochem Soc 160:A1016
Cho DH, Yashiro H, Sun YK, Myung ST, Electrochemical Properties of Polyaniline-Coated Li-Rich Nickel Manganese Oxide and Role of Polyaniline Coating Layer, (2014) J Electrochem Soc 161:A142
Thackeray MM, Kang SH, Johnson CS, Vaughey JT, Benedek R, Hackney S, Li2MnO3-stabilized LiMO2 (M = Mn, Ni, Co) electrodes for lithium-ion batteries,A (2007) J Mater Chem 17:3112
Xu B, Fell CR, Chi MF, Meng YS, Identifying surface structural changes in layered Li-excess nickel manganese oxides in high voltage lithium ion batteries: A joint experimental and theoretical study, (2011) Energy Environ Sci 4:2223
Lee HJ, Park YJ, Synthesis of Li[Ni0.2Li0.2Mn0.6]O2 nano-particles and their surface modification using a polydopamine layer, (2013) J Power Sources 244:222
Lee JB, Kumar PS, Moudgil BM, Singh RK, Electrochemical enhancement of LiFePO4 as a cathode material by incorporating Cu flakes for lithium ion rechargeable battery, (2013) Solid State Ionics 231:18
Zhou J, Liu BH, Li ZP, Nanostructure optimization of LiFePO4/carbon aerogel composites for performance enhancement, (2013) Solid State Ionics 244:23
Zang M, Jiao LF, Yuan HT, Wang YM, Guo J, Zhao M, Wang W, Zhou XD, The preparation and characterization of olivine LiFePO4/C doped with MoO3 by a solution method, (2006) Solid State Ionics 177:3309
Kim CH, Park YJ, Electrochemical performance of polydopamine-assisted Li[Ni1/3Co1/3Mn1/3]O2/Ketjenblack cathodes, (2014) Solid State Ionics 268:210
Noh HK, Park HS, Jeong HY, Lee SU, Song HK, Doubling the capacity of lithium manganese oxide spinel by a flexible skinny graphitic layer, (2014) Angew Chem 53:1
Savut Jana S, Nurgul S, Shi X, Xia H, Pang H, Improvement of electrochemical performance of LiNi0.8Co0.1Mn0.1O2 cathode material by graphene nanosheets modification, (2014) Electrochim Acta 149:86
Song B, Lai MO, Liu Z, Liu H, Lu L, Graphene-based surface modification on layered Li-rich cathode for high-performance Li-ion batteries, (2013) J Mater Chem 1:9954
Song B, Zhou C, Chen Y, Liu Z, Lai MO, Xue J, Lu L, Role of carbon coating in improving electrochemical performance of Li-rich Li(Li0.2Mn0.54Ni0.13 Co0.13)O2 cathode, (2014) RSC Adv 4:44244
Fey GT-K, Muralidharan P, Lu C-Z, Cho Y-D, Surface modification of LiNi0.8Co0.2O2 with La2O3 for lithium-ion batteries, (2005) Solid State Ionics 176:2759
This research was supported by Basic Science Research Program through the National Research Foundation of Korea (NRF) funded by the Ministry of Science, ICT and Future Planning (No.2014R1A2A2A01003542) and by the National Strategic R&D Program for Industrial Technology (10043868), funded by the Ministry of Trade, Industry and Energy (MOTIE).
MH performed the synthesis and characterization in this study. YJ gave advice and guided the experiment. Both authors read and approved the final manuscript.
The authors declare that they have no competing financial interests.